#------------------------------------------------------------------------------
#$Date: 2016-03-22 11:49:31 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178918 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/47/4114707.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4114707
loop_
_publ_author_name
'Svilen Bobev'
'Slavi C. Sevov'
_publ_section_title
;
 Naked Clusters of 56 Tin Atoms in the Solid State
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              3359
_journal_page_last               3365
_journal_paper_doi               10.1021/ja012549j
_journal_volume                  124
_journal_year                    2002
_chemical_formula_moiety         Ba16Na204Sn309.48
_chemical_formula_sum            'Ba16 Na204 Sn309.48'
_chemical_formula_weight         43619.58
_chemical_name_common            Ba16Na204Sn309.48
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           216
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           shelxl-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   25.1998(6)
_cell_length_b                   25.1998(6)
_cell_length_c                   25.1998(6)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      13.82
_cell_measurement_theta_min      12.88
_cell_volume                     16002.6(7)
_computing_cell_refinement       CAD4_(Enraf-Nonius,_1977)
_computing_data_collection       CAD4_(Enraf-Nonius,_1977)
_computing_data_reduction        SDS_Package_(Enraf-Nonius,_1985)
_computing_molecular_graphics    'SHELXTL (Siemens, 1994)'
_computing_publication_material  'SHELXTL (Siemens, 1994)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  Enraf_Nonius_CAD4
_diffrn_measurement_method       omega-2theta
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           Mok\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0482
_diffrn_reflns_av_sigmaI/netI    0.0427
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2013
_diffrn_reflns_theta_full        24.97
_diffrn_reflns_theta_max         24.97
_diffrn_reflns_theta_min         2.29
_diffrn_standards_interval_count 200
_diffrn_standards_interval_time  120
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    12.929
_exptl_absorpt_correction_T_max  0.3580
_exptl_absorpt_correction_T_min  0.3060
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   'average of 3 psi-scans'
_exptl_crystal_colour            grey-metallic
_exptl_crystal_density_diffrn    4.526
_exptl_crystal_description       bar
_exptl_crystal_F_000             18614
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_refine_diff_density_max         3.153
_refine_diff_density_min         -1.297
_refine_diff_density_rms         0.216
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.0(7)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.070
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     95
_refine_ls_number_reflns         763
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.070
_refine_ls_R_factor_all          0.0442
_refine_ls_R_factor_gt           0.0363
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0469P)²+435.8225P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0858
_refine_ls_wR_factor_ref         0.0894
_reflns_number_gt                673
_reflns_number_total             763
_reflns_threshold_expression     >2sigma(i)
_cod_data_source_file            ja012549j_2.cif
_cod_data_source_block           "'CAD4(1)'"
_cod_database_code               4114707
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, z'
'-y, -x, z'
'y, -x, -z'
'-y, x, -z'
'x, z, y'
'-x, z, -y'
'-x, -z, y'
'x, -z, -y'
'z, y, x'
'z, -y, -x'
'-z, y, -x'
'-z, -y, x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, z+1/2'
'-y, -x+1/2, z+1/2'
'y, -x+1/2, -z+1/2'
'-y, x+1/2, -z+1/2'
'x, z+1/2, y+1/2'
'-x, z+1/2, -y+1/2'
'-x, -z+1/2, y+1/2'
'x, -z+1/2, -y+1/2'
'z, y+1/2, x+1/2'
'z, -y+1/2, -x+1/2'
'-z, y+1/2, -x+1/2'
'-z, -y+1/2, x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, z+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, -x, -z+1/2'
'-y+1/2, x, -z+1/2'
'x+1/2, z, y+1/2'
'-x+1/2, z, -y+1/2'
'-x+1/2, -z, y+1/2'
'x+1/2, -z, -y+1/2'
'z+1/2, y, x+1/2'
'z+1/2, -y, -x+1/2'
'-z+1/2, y, -x+1/2'
'-z+1/2, -y, x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, z'
'-y+1/2, -x+1/2, z'
'y+1/2, -x+1/2, -z'
'-y+1/2, x+1/2, -z'
'x+1/2, z+1/2, y'
'-x+1/2, z+1/2, -y'
'-x+1/2, -z+1/2, y'
'x+1/2, -z+1/2, -y'
'z+1/2, y+1/2, x'
'z+1/2, -y+1/2, -x'
'-z+1/2, y+1/2, -x'
'-z+1/2, -y+1/2, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sn1 Sn 0.04884(8) 0.04884(8) 0.04884(8) 0.0316(8) Uani 1 6 d S
Sn2 Sn 0.82118(8) 0.82118(8) 0.82118(8) 0.0436(10) Uani 1 6 d S
Sn3 Sn 0.04066(6) 0.04066(6) 0.16321(8) 0.0302(4) Uani 1 2 d S
Sn4 Sn 0.11096(6) 0.11096(6) 0.75628(9) 0.0405(5) Uani 1 2 d S
Sn5 Sn 0.49842(7) 0.21602(5) 0.63500(5) 0.0351(4) Uani 1 1 d .
Sn6 Sn 0.5761(2) 0.5761(2) 0.5761(2) 0.055(5) Uani 0.392(17) 6 d SP
Sn7A Sn 0.45934(11) 0.45934(11) 0.37856(19) 0.0624(16) Uani 0.831(16) 2 d SP
Sn7B Sn 0.0605(14) 0.4753(13) 0.1044(13) 0.0624(16) Uani 0.084(8) 1 d P
Sn8 Sn 0.1961(3) 0.1961(3) 0.1961(3) 0.154(17) Uani 0.54(5) 6 d SP
Sn9 Sn 0.3038(4) 0.3038(4) 0.3038(4) 0.21(3) Uani 0.44(6) 6 d SP
Sn10 Sn 0.244(3) 0.3009(5) 0.1708(6) 0.24(3) Uani 0.164(15) 1 d P
Ba1 Ba 0.90422(7) 0.90422(7) 0.90422(7) 0.0348(7) Uani 1 6 d S
Na1 Na 0.5000 0.5000 0.5000 0.000(5) Uani 1 24 d S
Na2 Na 0.6849(14) 0.6849(14) 0.6849(14) 0.15(2) Uani 1 6 d S
Na3 Na 0.1313(7) 0.1313(7) 0.1313(7) 0.074(7) Uani 1 6 d S
Na4 Na 0.2734(10) 0.0000 0.0000 0.19(2) Uani 1 4 d S
Na5 Na 0.5820(9) 0.2500 0.2500 0.060(6) Uani 1 4 d S
Na6 Na 0.0623(15) 0.2500 0.2500 0.096(10) Uani 1 4 d S
Na7 Na 0.1021(4) 0.1021(4) 0.2844(6) 0.062(4) Uani 1 2 d S
Na8 Na 0.1538(5) 0.1538(5) 0.5306(7) 0.081(5) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
na na 0.0362 0.0249 'international tables vol c tables 4.2.6.8 and 6.1.1.4'
sn sn -0.6537 1.4246 'international tables vol c tables 4.2.6.8 and 6.1.1.4'
ba ba -0.3244 2.2819 'international tables vol c tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sn3 Sn1 Sn3 97.84(10) 5 9
Sn3 Sn1 Sn3 97.84(10) 5 .
Sn3 Sn1 Sn3 97.84(10) 9 .
Sn3 Sn1 Na3 60.51(7) 5 .
Sn3 Sn1 Na3 60.51(7) 9 .
Sn3 Sn1 Na3 60.51(7) . .
Sn3 Sn1 Ba1 70.30(2) 5 3_646
Sn3 Sn1 Ba1 161.11(12) 9 3_646
Sn3 Sn1 Ba1 70.30(2) . 3_646
Na3 Sn1 Ba1 100.61(5) . 3_646
Sn3 Sn1 Ba1 70.30(2) 5 2_664
Sn3 Sn1 Ba1 70.30(2) 9 2_664
Sn3 Sn1 Ba1 161.11(12) . 2_664
Na3 Sn1 Ba1 100.61(5) . 2_664
Ba1 Sn1 Ba1 116.69(3) 3_646 2_664
Sn3 Sn1 Ba1 161.11(12) 5 4_466
Sn3 Sn1 Ba1 70.30(2) 9 4_466
Sn3 Sn1 Ba1 70.30(2) . 4_466
Na3 Sn1 Ba1 100.61(5) . 4_466
Ba1 Sn1 Ba1 116.69(3) 3_646 4_466
Ba1 Sn1 Ba1 116.69(3) 2_664 4_466
Sn4 Sn2 Sn4 108.25(8) 10_656 2_665
Sn4 Sn2 Sn4 108.25(8) 10_656 6_566
Sn4 Sn2 Sn4 108.25(8) 2_665 6_566
Sn4 Sn2 Na2 59.5(8) 10_656 51_656
Sn4 Sn2 Na2 125.83(5) 2_665 51_656
Sn4 Sn2 Na2 125.87(5) 6_566 51_656
Sn4 Sn2 Na2 125.83(5) 10_656 74_665
Sn4 Sn2 Na2 59.5(8) 2_665 74_665
Sn4 Sn2 Na2 125.87(5) 6_566 74_665
Na2 Sn2 Na2 84.8(12) 51_656 74_665
Sn4 Sn2 Na2 125.85(5) 10_656 28_566
Sn4 Sn2 Na2 125.85(5) 2_665 28_566
Sn4 Sn2 Na2 59.6(8) 6_566 28_566
Na2 Sn2 Na2 84.8(13) 51_656 28_566
Na2 Sn2 Na2 84.8(13) 74_665 28_566
Sn4 Sn2 Na5 66.86(12) 10_656 50_665
Sn4 Sn2 Na5 66.86(12) 2_665 50_665
Sn4 Sn2 Na5 170.2(3) 6_566 50_665
Na2 Sn2 Na5 60.0(2) 51_656 50_665
Na2 Sn2 Na5 60.0(2) 74_665 50_665
Na2 Sn2 Na5 130.3(9) 28_566 50_665
Sn4 Sn2 Na5 66.86(12) 10_656 34_656
Sn4 Sn2 Na5 170.2(3) 2_665 34_656
Sn4 Sn2 Na5 66.86(12) 6_566 34_656
Na2 Sn2 Na5 60.0(2) 51_656 34_656
Na2 Sn2 Na5 130.3(9) 74_665 34_656
Na2 Sn2 Na5 60.0(2) 28_566 34_656
Na5 Sn2 Na5 116.54(16) 50_665 34_656
Sn4 Sn2 Na5 170.2(3) 10_656 78_566
Sn4 Sn2 Na5 66.86(12) 2_665 78_566
Sn4 Sn2 Na5 66.86(12) 6_566 78_566
Na2 Sn2 Na5 130.3(9) 51_656 78_566
Na2 Sn2 Na5 60.0(2) 74_665 78_566
Na2 Sn2 Na5 60.0(2) 28_566 78_566
Na5 Sn2 Na5 116.54(16) 50_665 78_566
Na5 Sn2 Na5 116.54(17) 34_656 78_566
Sn4 Sn2 Ba1 69.33(8) 10_656 .
Sn4 Sn2 Ba1 69.33(8) 2_665 .
Sn4 Sn2 Ba1 69.33(8) 6_566 .
Na2 Sn2 Ba1 128.9(8) 51_656 .
Na2 Sn2 Ba1 128.9(8) 74_665 .
Na2 Sn2 Ba1 128.9(8) 28_566 .
Na5 Sn2 Ba1 100.9(3) 50_665 .
Na5 Sn2 Ba1 100.9(3) 34_656 .
Na5 Sn2 Ba1 100.9(3) 78_566 .
Sn1 Sn3 Sn3 95.77(7) . 2
Sn1 Sn3 Sn5 114.88(5) . 77_445
Sn3 Sn3 Sn5 108.50(5) 2 77_445
Sn1 Sn3 Sn5 114.88(5) . 89_445
Sn3 Sn3 Sn5 108.50(5) 2 89_445
Sn5 Sn3 Sn5 112.62(9) 77_445 89_445
Sn1 Sn3 Na4 158.2(2) . 9
Sn3 Sn3 Na4 62.5(2) 2 9
Sn5 Sn3 Na4 75.13(12) 77_445 9
Sn5 Sn3 Na4 75.13(12) 89_445 9
Sn1 Sn3 Na3 70.3(4) . .
Sn3 Sn3 Na3 166.0(4) 2 .
Sn5 Sn3 Na3 78.6(2) 77_445 .
Sn5 Sn3 Na3 78.6(2) 89_445 .
Na4 Sn3 Na3 131.5(5) 9 .
Sn1 Sn3 Na7 138.6(3) . .
Sn3 Sn3 Na7 125.6(3) 2 .
Sn5 Sn3 Na7 56.31(4) 77_445 .
Sn5 Sn3 Na7 56.31(4) 89_445 .
Na4 Sn3 Na7 63.2(3) 9 .
Na3 Sn3 Na7 68.3(5) . .
Sn5 Sn4 Sn5 109.73(9) 78_456 90_546
Sn5 Sn4 Sn2 107.38(7) 78_456 2_665
Sn5 Sn4 Sn2 107.38(7) 90_546 2_665
Sn5 Sn4 Na2 124.59(13) 78_456 73_445
Sn5 Sn4 Na2 124.55(13) 90_546 73_445
Sn2 Sn4 Na2 68.4(10) 2_665 73_445
Sn5 Sn4 Na8 63.8(3) 78_456 33_545
Sn5 Sn4 Na8 126.7(3) 90_546 33_545
Sn2 Sn4 Na8 125.4(3) 2_665 33_545
Na2 Sn4 Na8 74.9(8) 73_445 33_545
Sn5 Sn4 Na8 126.7(3) 78_456 53_455
Sn5 Sn4 Na8 63.8(3) 90_546 53_455
Sn2 Sn4 Na8 125.4(3) 2_665 53_455
Na2 Sn4 Na8 74.8(8) 73_445 53_455
Na8 Sn4 Na8 78.9(7) 33_545 53_455
Sn5 Sn4 Na5 67.3(3) 78_456 29_545
Sn5 Sn4 Na5 168.62(9) 90_546 29_545
Sn2 Sn4 Na5 64.6(3) 2_665 29_545
Na2 Sn4 Na5 61.5(4) 73_445 29_545
Na8 Sn4 Na5 62.7(4) 33_545 29_545
Na8 Sn4 Na5 127.2(3) 53_455 29_545
Sn5 Sn4 Na5 168.62(9) 78_456 49_455
Sn5 Sn4 Na5 67.3(3) 90_546 49_455
Sn2 Sn4 Na5 64.6(3) 2_665 49_455
Na2 Sn4 Na5 61.5(4) 73_445 49_455
Na8 Sn4 Na5 127.2(3) 33_545 49_455
Na8 Sn4 Na5 62.7(4) 53_455 49_455
Na5 Sn4 Na5 113.4(7) 29_545 49_455
Sn5 Sn4 Ba1 71.78(5) 78_456 2_665
Sn5 Sn4 Ba1 71.78(5) 90_546 2_665
Sn2 Sn4 Ba1 64.19(9) 2_665 2_665
Na2 Sn4 Ba1 132.6(10) 73_445 2_665
Na8 Sn4 Ba1 135.4(3) 33_545 2_665
Na8 Sn4 Ba1 135.4(3) 53_455 2_665
Na5 Sn4 Ba1 97.03(7) 29_545 2_665
Na5 Sn4 Ba1 97.03(7) 49_455 2_665
Sn5 Sn5 Sn4 108.49(5) 41_545 60_565
Sn5 Sn5 Sn3 104.66(4) 41_545 57
Sn4 Sn5 Sn3 106.55(7) 60_565 57
Sn5 Sn5 Na7 123.9(3) 41_545 57
Sn4 Sn5 Na7 125.7(3) 60_565 57
Sn3 Sn5 Na7 74.95(19) 57 57
Sn5 Sn5 Na8 125.8(3) 41_545 31_655
Sn4 Sn5 Na8 66.0(3) 60_565 31_655
Sn3 Sn5 Na8 129.2(3) 57 31_655
Na7 Sn5 Na8 72.2(4) 57 31_655
Sn5 Sn5 Na6 65.06(14) 41_545 49
Sn4 Sn5 Na6 124.2(5) 60_565 49
Sn3 Sn5 Na6 129.1(5) 57 49
Na7 Sn5 Na6 72.8(5) 57 49
Na8 Sn5 Na6 75.0(3) 31_655 49
Sn5 Sn5 Na5 66.62(9) 41_545 26_655
Sn4 Sn5 Na5 65.3(3) 60_565 26_655
Sn3 Sn5 Na5 163.2(2) 57 26_655
Na7 Sn5 Na5 121.9(3) 57 26_655
Na8 Sn5 Na5 62.7(3) 31_655 26_655
Na6 Sn5 Na5 61.9(6) 49 26_655
Sn5 Sn5 Na4 158.0(4) 41_545 53
Sn4 Sn5 Na4 74.01(8) 60_565 53
Sn3 Sn5 Na4 55.0(3) 57 53
Na7 Sn5 Na4 63.1(3) 57 53
Na8 Sn5 Na4 75.7(5) 31_655 53
Na6 Sn5 Na4 132.5(4) 49 53
Na5 Sn5 Na4 130.3(3) 26_655 53
Sn5 Sn5 Ba1 68.70(2) 41_545 52_466
Sn4 Sn5 Ba1 64.21(6) 60_565 52_466
Sn3 Sn5 Ba1 70.63(6) 57 52_466
Na7 Sn5 Ba1 145.50(19) 57 52_466
Na8 Sn5 Ba1 130.0(3) 31_655 52_466
Na6 Sn5 Ba1 133.0(2) 49 52_466
Na5 Sn5 Ba1 92.6(2) 26_655 52_466
Na4 Sn5 Ba1 94.4(3) 53 52_466
Sn7B Sn6 Sn7B 69.4(15) 69 77
Sn7B Sn6 Sn7B 98.8(8) 69 89
Sn7B Sn6 Sn7B 34.1(15) 77 89
Sn7B Sn6 Sn7B 34.1(15) 69 49
Sn7B Sn6 Sn7B 98.8(8) 77 49
Sn7B Sn6 Sn7B 119.2(13) 89 49
Sn7B Sn6 Sn7B 98.8(8) 69 37
Sn7B Sn6 Sn7B 119.2(13) 77 37
Sn7B Sn6 Sn7B 98.8(8) 89 37
Sn7B Sn6 Sn7B 69.4(15) 49 37
Sn7B Sn6 Sn7B 119.2(13) 69 33
Sn7B Sn6 Sn7B 98.8(8) 77 33
Sn7B Sn6 Sn7B 69.4(15) 89 33
Sn7B Sn6 Sn7B 98.8(8) 49 33
Sn7B Sn6 Sn7B 34.1(15) 37 33
Sn7B Sn6 Na8 63.7(7) 69 57
Sn7B Sn6 Na8 113.0(8) 77 57
Sn7B Sn6 Na8 145.2(8) 89 57
Sn7B Sn6 Na8 63.7(7) 49 57
Sn7B Sn6 Na8 113.0(8) 37 57
Sn7B Sn6 Na8 145.2(8) 33 57
Sn7B Sn6 Na8 113.0(8) 69 73
Sn7B Sn6 Na8 63.7(7) 77 73
Sn7B Sn6 Na8 63.7(7) 89 73
Sn7B Sn6 Na8 145.2(8) 49 73
Sn7B Sn6 Na8 145.2(8) 37 73
Sn7B Sn6 Na8 113.0(8) 33 73
Na8 Sn6 Na8 94.2(5) 57 73
Sn7B Sn6 Na8 145.2(8) 69 29
Sn7B Sn6 Na8 145.2(8) 77 29
Sn7B Sn6 Na8 113.0(8) 89 29
Sn7B Sn6 Na8 113.0(8) 49 29
Sn7B Sn6 Na8 63.7(7) 37 29
Sn7B Sn6 Na8 63.7(7) 33 29
Na8 Sn6 Na8 94.2(5) 57 29
Na8 Sn6 Na8 94.2(5) 73 29
Sn7B Sn6 Sn7A 61.0(8) 69 7_665
Sn7B Sn6 Sn7A 9.1(8) 77 7_665
Sn7B Sn6 Sn7A 43.1(8) 89 7_665
Sn7B Sn6 Sn7A 91.8(7) 49 7_665
Sn7B Sn6 Sn7A 122.1(7) 37 7_665
Sn7B Sn6 Sn7A 105.8(7) 33 7_665
Na8 Sn6 Sn7A 104.73(17) 57 7_665
Na8 Sn6 Sn7A 66.9(3) 73 7_665
Na8 Sn6 Sn7A 153.78(8) 29 7_665
Sn7B Sn6 Sn7A 9.1(7) 69 8_656
Sn7B Sn6 Sn7A 61.0(8) 77 8_656
Sn7B Sn6 Sn7A 91.8(7) 89 8_656
Sn7B Sn6 Sn7A 43.1(8) 49 8_656
Sn7B Sn6 Sn7A 105.8(7) 37 8_656
Sn7B Sn6 Sn7A 122.1(7) 33 8_656
Na8 Sn6 Sn7A 66.9(3) 57 8_656
Na8 Sn6 Sn7A 104.72(17) 73 8_656
Na8 Sn6 Sn7A 153.78(8) 29 8_656
Sn7A Sn6 Sn7A 52.44(16) 7_665 8_656
Sn7B Sn6 Sn7A 105.8(7) 69 12_665
Sn7B Sn6 Sn7A 43.1(8) 77 12_665
Sn7B Sn6 Sn7A 9.1(8) 89 12_665
Sn7B Sn6 Sn7A 122.1(7) 49 12_665
Sn7B Sn6 Sn7A 91.8(7) 37 12_665
Sn7B Sn6 Sn7A 61.0(8) 33 12_665
Na8 Sn6 Sn7A 153.78(8) 57 12_665
Na8 Sn6 Sn7A 66.9(3) 73 12_665
Na8 Sn6 Sn7A 104.72(17) 29 12_665
Sn7A Sn6 Sn7A 52.06(18) 7_665 12_665
Sn7A Sn6 Sn7A 99.4(2) 8_656 12_665
Sn7B Sn7A Sn7B 111(4) 39 51
Sn7B Sn7A Sn7B 21.3(18) 39 35
Sn7B Sn7A Sn7B 96(3) 51 35
Sn7B Sn7A Sn7B 96(3) 39 71
Sn7B Sn7A Sn7B 21.3(18) 51 71
Sn7B Sn7A Sn7B 77.9(17) 35 71
Sn7B Sn7A Sn7A 32(2) 39 9
Sn7B Sn7A Sn7A 89(2) 51 9
Sn7B Sn7A Sn7A 10.4(9) 35 9
Sn7B Sn7A Sn7A 69.2(8) 71 9
Sn7B Sn7A Sn7A 89(2) 39 5
Sn7B Sn7A Sn7A 32(2) 51 5
Sn7B Sn7A Sn7A 69.2(9) 35 5
Sn7B Sn7A Sn7A 10.4(9) 71 5
Sn7A Sn7A Sn7A 60.0 9 5
Sn7B Sn7A Sn7A 95(2) 39 2_665
Sn7B Sn7A Sn7A 95(2) 51 2_665
Sn7B Sn7A Sn7A 112.1(9) 35 2_665
Sn7B Sn7A Sn7A 112.1(9) 71 2_665
Sn7A Sn7A Sn7A 119.999(1) 9 2_665
Sn7A Sn7A Sn7A 120.0 5 2_665
Sn7B Sn7A Sn7B 44(2) 39 91
Sn7B Sn7A Sn7B 73(2) 51 91
Sn7B Sn7A Sn7B 23.8(15) 35 91
Sn7B Sn7A Sn7B 54.3(7) 71 91
Sn7A Sn7A Sn7B 15.1(8) 9 91
Sn7A Sn7A Sn7B 45.5(8) 5 91
Sn7A Sn7A Sn7B 120.2(6) 2_665 91
Sn7B Sn7A Sn7B 73(2) 39 79
Sn7B Sn7A Sn7B 44(2) 51 79
Sn7B Sn7A Sn7B 54.3(7) 35 79
Sn7B Sn7A Sn7B 23.7(15) 71 79
Sn7A Sn7A Sn7B 45.5(8) 9 79
Sn7A Sn7A Sn7B 15.1(8) 5 79
Sn7A Sn7A Sn7B 120.2(6) 2_665 79
Sn7B Sn7A Sn7B 30.6(15) 91 79
Sn7B Sn7A Na4 122(2) 39 81
Sn7B Sn7A Na4 122(2) 51 81
Sn7B Sn7A Na4 141.0(8) 35 81
Sn7B Sn7A Na4 141.0(8) 71 81
Sn7A Sn7A Na4 149.35(5) 9 81
Sn7A Sn7A Na4 149.35(5) 5 81
Sn7A Sn7A Na4 61.3(2) 2_665 81
Sn7B Sn7A Na4 164.5(8) 91 81
Sn7B Sn7A Na4 164.5(8) 79 81
Sn7B Sn7A Sn7B 81(3) 39 52_565
Sn7B Sn7A Sn7B 100(2) 51 52_565
Sn7B Sn7A Sn7B 97.9(15) 35 52_565
Sn7B Sn7A Sn7B 113.6(11) 71 52_565
Sn7A Sn7A Sn7B 106.3(7) 9 52_565
Sn7A Sn7A Sn7B 119.3(5) 5 52_565
Sn7A Sn7A Sn7B 14.5(7) 2_665 52_565
Sn7B Sn7A Sn7B 108.4(10) 91 52_565
Sn7B Sn7A Sn7B 115.2(10) 79 52_565
Na4 Sn7A Sn7B 70.0(6) 81 52_565
Sn7B Sn7A Sn7B 100(2) 39 40_655
Sn7B Sn7A Sn7B 81(3) 51 40_655
Sn7B Sn7A Sn7B 113.6(11) 35 40_655
Sn7B Sn7A Sn7B 97.9(15) 71 40_655
Sn7A Sn7A Sn7B 119.3(5) 9 40_655
Sn7A Sn7A Sn7B 106.3(7) 5 40_655
Sn7A Sn7A Sn7B 14.5(7) 2_665 40_655
Sn7B Sn7A Sn7B 115.2(10) 91 40_655
Sn7B Sn7A Sn7B 108.4(10) 79 40_655
Na4 Sn7A Sn7B 70.0(6) 81 40_655
Sn7B Sn7A Sn7B 24.0(13) 52_565 40_655
Sn7A Sn7B Sn7B 34(2) 51 86
Sn7A Sn7B Sn7B 148(2) 51 21
Sn7B Sn7B Sn7B 119.994(8) 86 21
Sn7A Sn7B Sn7A 138(3) 51 56
Sn7B Sn7B Sn7A 110.8(8) 86 56
Sn7B Sn7B Sn7A 10.4(9) 21 56
Sn7A Sn7B Sn7B 66(3) 51 84
Sn7B Sn7B Sn7B 33.3(16) 86 84
Sn7B Sn7B Sn7B 86.6(16) 21 84
Sn7A Sn7B Sn7B 77.6(11) 56 84
Sn7A Sn7B Sn7B 124(3) 51 30
Sn7B Sn7B Sn7B 93.3(16) 86 30
Sn7B Sn7B Sn7B 26.7(16) 21 30
Sn7A Sn7B Sn7B 18.2(11) 56 30
Sn7B Sn7B Sn7B 59.998(1) 84 30
Sn7A Sn7B Sn6 138(3) 51 49_454
Sn7B Sn7B Sn6 141.0(7) 86 49_454
Sn7B Sn7B Sn6 72.9(8) 21 49_454
Sn7A Sn7B Sn6 83.1(13) 56 49_454
Sn7B Sn7B Sn6 135.3(11) 84 49_454
Sn7B Sn7B Sn6 93.7(19) 30 49_454
Sn7A Sn7B Sn7B 91(2) 51 44
Sn7B Sn7B Sn7B 59.997(2) 86 44
Sn7B Sn7B Sn7B 59.997(5) 21 44
Sn7A Sn7B Sn7B 51.0(8) 56 44
Sn7B Sn7B Sn7B 26.7(16) 84 44
Sn7B Sn7B Sn7B 33.3(16) 30 44
Sn6 Sn7B Sn7B 119.0(7) 49_454 44
Sn7A Sn7B Sn7A 76(2) 51 58
Sn7B Sn7B Sn7A 45.5(8) 86 58
Sn7B Sn7B Sn7A 74.7(8) 21 58
Sn7A Sn7B Sn7A 65.3(7) 56 58
Sn7B Sn7B Sn7A 12.6(9) 84 58
Sn7B Sn7B Sn7A 48.1(9) 30 58
Sn6 Sn7B Sn7A 131.6(12) 49_454 58
Sn7B Sn7B Sn7A 15.1(8) 44 58
Sn7A Sn7B Na8 121(2) 51 9
Sn7B Sn7B Na8 151.8(7) 86 9
Sn7B Sn7B Na8 74.9(7) 21 9
Sn7A Sn7B Na8 81.1(11) 56 9
Sn7B Sn7B Na8 148.3(13) 84 9
Sn7B Sn7B Na8 99(2) 30 9
Sn6 Sn7B Na8 63.5(8) 49_454 9
Sn7B Sn7B Na8 128.4(6) 44 9
Sn7A Sn7B Na8 137.6(12) 58 9
Sn7A Sn7B Sn7B 85(2) 51 85_455
Sn7B Sn7B Sn7B 90.001(2) 86 85_455
Sn7B Sn7B Sn7B 119.998(3) 21 85_455
Sn7A Sn7B Sn7B 127.4(8) 56 85_455
Sn7B Sn7B Sn7B 108.5(8) 84 85_455
Sn7B Sn7B Sn7B 125.19(7) 30 85_455
Sn6 Sn7B Sn7B 55.3(7) 49_454 85_455
Sn7B Sn7B Sn7B 119.998(3) 44 85_455
Sn7A Sn7B Sn7B 117.6(6) 58 85_455
Na8 Sn7B Sn7B 103.1(6) 9 85_455
Sn7A Sn7B Sn7A 70(2) 51 52_465
Sn7B Sn7B Sn7A 78.0(7) 86 52_465
Sn7B Sn7B Sn7A 133.4(7) 21 52_465
Sn7A Sn7B Sn7A 139.6(13) 56 52_465
Sn7B Sn7B Sn7A 101.3(16) 84 52_465
Sn7B Sn7B Sn7A 133.2(5) 30 52_465
Sn6 Sn7B Sn7A 69.4(7) 49_454 52_465
Sn7B Sn7B Sn7A 118.6(5) 44 52_465
Sn7A Sn7B Sn7A 112.2(10) 58 52_465
Na8 Sn7B Sn7A 110.1(9) 9 52_465
Sn7B Sn7B Sn7A 14.5(7) 85_455 52_465
Sn10 Sn8 Sn10 36(2) 66 74
Sn10 Sn8 Sn10 109.4(11) 66 86
Sn10 Sn8 Sn10 76.6(15) 74 86
Sn10 Sn8 Sn10 76.6(15) 66 58
Sn10 Sn8 Sn10 109.4(11) 74 58
Sn10 Sn8 Sn10 135(3) 86 58
Sn10 Sn8 Sn10 135(3) 66 30
Sn10 Sn8 Sn10 109.4(11) 74 30
Sn10 Sn8 Sn10 36(2) 86 30
Sn10 Sn8 Sn10 109.4(11) 58 30
Sn10 Sn8 Sn10 109.4(11) 66 46
Sn10 Sn8 Sn10 135(3) 74 46
Sn10 Sn8 Sn10 109.4(11) 86 46
Sn10 Sn8 Sn10 36(2) 58 46
Sn10 Sn8 Sn10 76.6(15) 30 46
Sn10 Sn8 Sn9 23.0(13) 66 28
Sn10 Sn8 Sn9 23.0(13) 74 28
Sn10 Sn8 Sn9 87.4(6) 86 28
Sn10 Sn8 Sn9 87.4(6) 58 28
Sn10 Sn8 Sn9 112.7(15) 30 28
Sn10 Sn8 Sn9 112.7(15) 46 28
Sn10 Sn8 Sn9 87.4(6) 66 74
Sn10 Sn8 Sn9 112.7(15) 74 74
Sn10 Sn8 Sn9 112.7(15) 86 74
Sn10 Sn8 Sn9 23.0(13) 58 74
Sn10 Sn8 Sn9 87.4(6) 30 74
Sn10 Sn8 Sn9 23.0(13) 46 74
Sn9 Sn8 Sn9 89.9(5) 28 74
Sn10 Sn8 Sn9 112.7(15) 66 51
Sn10 Sn8 Sn9 87.4(6) 74 51
Sn10 Sn8 Sn9 23.0(13) 86 51
Sn10 Sn8 Sn9 112.7(15) 58 51
Sn10 Sn8 Sn9 23.0(13) 30 51
Sn10 Sn8 Sn9 87.4(6) 46 51
Sn9 Sn8 Sn9 89.9(5) 28 51
Sn9 Sn8 Sn9 89.9(5) 74 51
Sn10 Sn8 Na3 109.5(11) 66 .
Sn10 Sn8 Na3 109.5(11) 74 .
Sn10 Sn8 Na3 109.5(11) 86 .
Sn10 Sn8 Na3 109.5(11) 58 .
Sn10 Sn8 Na3 109.5(11) 30 .
Sn10 Sn8 Na3 109.5(11) 46 .
Sn9 Sn8 Na3 125.3(3) 28 .
Sn9 Sn8 Na3 125.3(3) 74 .
Sn9 Sn8 Na3 125.3(3) 51 .
Sn10 Sn8 Sn10 23.0(14) 66 9
Sn10 Sn8 Sn10 49(2) 74 9
Sn10 Sn8 Sn10 108.3(11) 86 9
Sn10 Sn8 Sn10 60.4(16) 58 9
Sn10 Sn8 Sn10 121.6(12) 30 9
Sn10 Sn8 Sn10 89.0(6) 46 9
Sn9 Sn8 Sn10 27.2(12) 28 9
Sn9 Sn8 Sn10 66.2(12) 74 9
Sn9 Sn8 Sn10 102.3(5) 51 9
Na3 Sn8 Sn10 128.5(5) . 9
Sn10 Sn8 Sn10 49(2) 66 13
Sn10 Sn8 Sn10 23.0(14) 74 13
Sn10 Sn8 Sn10 60.4(16) 86 13
Sn10 Sn8 Sn10 108.3(11) 58 13
Sn10 Sn8 Sn10 89.0(6) 30 13
Sn10 Sn8 Sn10 121.6(12) 46 13
Sn9 Sn8 Sn10 27.2(12) 28 13
Sn9 Sn8 Sn10 102.3(5) 74 13
Sn9 Sn8 Sn10 66.2(12) 51 13
Na3 Sn8 Sn10 128.5(5) . 13
Sn10 Sn8 Sn10 51.8(19) 9 13
Sn10 Sn9 Sn10 71.7(14) 79 71
Sn10 Sn9 Sn10 113.2(12) 79 35
Sn10 Sn9 Sn10 43.5(19) 71 35
Sn10 Sn9 Sn10 43.5(19) 79 39
Sn10 Sn9 Sn10 113.2(12) 71 39
Sn10 Sn9 Sn10 146(3) 35 39
Sn10 Sn9 Sn10 146(3) 79 91
Sn10 Sn9 Sn10 113.2(12) 71 91
Sn10 Sn9 Sn10 71.7(14) 35 91
Sn10 Sn9 Sn10 113.2(13) 39 91
Sn10 Sn9 Sn10 113.2(12) 79 51
Sn10 Sn9 Sn10 146(3) 71 51
Sn10 Sn9 Sn10 113.2(12) 35 51
Sn10 Sn9 Sn10 71.7(14) 39 51
Sn10 Sn9 Sn10 43.5(19) 91 51
Sn10 Sn9 Sn8 28.3(14) 79 51
Sn10 Sn9 Sn8 87.0(8) 71 51
Sn10 Sn9 Sn8 118.2(17) 35 51
Sn10 Sn9 Sn8 28.3(14) 39 51
Sn10 Sn9 Sn8 118.2(17) 91 51
Sn10 Sn9 Sn8 87.0(8) 51 51
Sn10 Sn9 Sn8 87.0(8) 79 74
Sn10 Sn9 Sn8 28.3(14) 71 74
Sn10 Sn9 Sn8 28.3(14) 35 74
Sn10 Sn9 Sn8 118.2(17) 39 74
Sn10 Sn9 Sn8 87.0(8) 91 74
Sn10 Sn9 Sn8 118.2(17) 51 74
Sn8 Sn9 Sn8 90.1(5) 51 74
Sn10 Sn9 Sn8 118.2(17) 79 28
Sn10 Sn9 Sn8 118.2(17) 71 28
Sn10 Sn9 Sn8 87.0(8) 35 28
Sn10 Sn9 Sn8 87.0(8) 39 28
Sn10 Sn9 Sn8 28.3(14) 91 28
Sn10 Sn9 Sn8 28.3(14) 51 28
Sn8 Sn9 Sn8 90.1(5) 51 28
Sn8 Sn9 Sn8 90.1(5) 74 28
Sn10 Sn9 Sn10 29.6(18) 79 96
Sn10 Sn9 Sn10 55.2(11) 71 96
Sn10 Sn9 Sn10 89.0(8) 35 96
Sn10 Sn9 Sn10 60(2) 39 96
Sn10 Sn9 Sn10 123.8(14) 91 96
Sn10 Sn9 Sn10 111.5(14) 51 96
Sn8 Sn9 Sn10 32.0(10) 51 96
Sn8 Sn9 Sn10 60.9(11) 74 96
Sn8 Sn9 Sn10 102.0(6) 28 96
Sn10 Sn9 Sn10 55.2(11) 79 56
Sn10 Sn9 Sn10 29.6(18) 71 56
Sn10 Sn9 Sn10 60(2) 35 56
Sn10 Sn9 Sn10 89.0(8) 39 56
Sn10 Sn9 Sn10 111.5(14) 91 56
Sn10 Sn9 Sn10 123.8(14) 51 56
Sn8 Sn9 Sn10 60.9(11) 51 56
Sn8 Sn9 Sn10 32.0(10) 74 56
Sn8 Sn9 Sn10 102.0(6) 28 56
Sn10 Sn9 Sn10 30(2) 96 56
Sn10 Sn9 Sn10 111.5(14) 79 44
Sn10 Sn9 Sn10 60(2) 71 44
Sn10 Sn9 Sn10 29.6(18) 35 44
Sn10 Sn9 Sn10 123.8(14) 39 44
Sn10 Sn9 Sn10 55.2(11) 91 44
Sn10 Sn9 Sn10 89.0(8) 51 44
Sn8 Sn9 Sn10 102.0(6) 51 44
Sn8 Sn9 Sn10 32.0(10) 74 44
Sn8 Sn9 Sn10 60.9(11) 28 44
Sn10 Sn9 Sn10 82.1(9) 96 44
Sn10 Sn9 Sn10 58.7(13) 56 44
Sn10 Sn10 Sn9 68.3(9) 44 51
Sn10 Sn10 Sn10 119.994(4) 44 86
Sn9 Sn10 Sn10 54.2(7) 51 86
Sn10 Sn10 Sn8 72.2(10) 44 74
Sn9 Sn10 Sn8 128.8(12) 51 74
Sn10 Sn10 Sn8 133.1(7) 86 74
Sn10 Sn10 Sn10 120.003(9) 44 13
Sn9 Sn10 Sn10 131.3(11) 51 13
Sn10 Sn10 Sn10 89.999(10) 86 13
Sn8 Sn10 Sn10 51.7(7) 74 13
Sn10 Sn10 Sn10 37.4(9) 44 84
Sn9 Sn10 Sn10 33.4(6) 51 84
Sn10 Sn10 Sn10 82.6(9) 86 84
Sn8 Sn10 Sn10 97.4(11) 74 84
Sn10 Sn10 Sn10 124.93(8) 13 84
Sn10 Sn10 Sn10 97.4(9) 44 30
Sn9 Sn10 Sn10 33.4(6) 51 30
Sn10 Sn10 Sn10 22.6(9) 86 30
Sn8 Sn10 Sn10 130.3(9) 74 30
Sn10 Sn10 Sn10 102.8(5) 13 30
Sn10 Sn10 Sn10 59.998(3) 84 30
Sn10 Sn10 Sn10 134.6(4) 44 74
Sn9 Sn10 Sn10 99(3) 51 74
Sn10 Sn10 Sn10 52(3) 86 74
Sn8 Sn10 Sn10 86(3) 74 74
Sn10 Sn10 Sn10 38(3) 13 74
Sn10 Sn10 Sn10 112(2) 84 74
Sn10 Sn10 Sn10 67(3) 30 74
Sn10 Sn10 Sn10 59.996(2) 44 21
Sn9 Sn10 Sn10 17.1(16) 51 21
Sn10 Sn10 Sn10 59.998(1) 86 21
Sn8 Sn10 Sn10 112.2(13) 74 21
Sn10 Sn10 Sn10 119.998(5) 13 21
Sn10 Sn10 Sn10 22.6(9) 84 21
Sn10 Sn10 Sn10 37.4(9) 30 21
Sn10 Sn10 Sn10 95(2) 74 21
Sn10 Sn10 Sn10 101.1(10) 44 56
Sn9 Sn10 Sn10 127.5(13) 51 56
Sn10 Sn10 Sn10 100.8(6) 86 56
Sn8 Sn10 Sn10 35.3(5) 74 56
Sn10 Sn10 Sn10 18.9(10) 13 56
Sn10 Sn10 Sn10 110.6(8) 84 56
Sn10 Sn10 Sn10 107.4(2) 30 56
Sn10 Sn10 Sn10 51(4) 74 56
Sn10 Sn10 Sn10 112.3(5) 21 56
Sn10 Sn10 Sn10 41.1(10) 44 35
Sn9 Sn10 Sn10 94.6(11) 51 35
Sn10 Sn10 Sn10 124.51(13) 86 35
Sn8 Sn10 Sn10 35.3(5) 74 35
Sn10 Sn10 Sn10 78.9(10) 13 35
Sn10 Sn10 Sn10 62.3(8) 84 35
Sn10 Sn10 Sn10 108.3(6) 30 35
Sn10 Sn10 Sn10 101(3) 74 35
Sn10 Sn10 Sn10 79.2(6) 21 35
Sn10 Sn10 Sn10 60.001(2) 56 35
Sn10 Sn10 Sn8 118.5(6) 44 .
Sn9 Sn10 Sn8 65.8(12) 51 .
Sn10 Sn10 Sn8 23.9(11) 86 .
Sn8 Sn10 Sn8 109.2(11) 74 .
Sn10 Sn10 Sn8 69.9(12) 13 .
Sn10 Sn10 Sn8 84.5(14) 84 .
Sn10 Sn10 Sn8 33.4(17) 30 .
Sn10 Sn10 Sn8 33.6(16) 74 .
Sn10 Sn10 Sn8 64.1(9) 21 .
Sn10 Sn10 Sn8 77.8(16) 56 .
Sn10 Sn10 Sn8 106.3(9) 35 .
Sn2 Ba1 Sn4 46.48(5) . 10_656
Sn2 Ba1 Sn4 46.48(5) . 2_665
Sn4 Ba1 Sn4 77.80(7) 10_656 2_665
Sn2 Ba1 Sn4 46.48(5) . 6_566
Sn4 Ba1 Sn4 77.80(7) 10_656 6_566
Sn4 Ba1 Sn4 77.80(7) 2_665 6_566
Sn2 Ba1 Sn5 76.18(5) . 92_566
Sn4 Ba1 Sn5 74.76(4) 10_656 92_566
Sn4 Ba1 Sn5 44.01(3) 2_665 92_566
Sn4 Ba1 Sn5 119.24(8) 6_566 92_566
Sn2 Ba1 Sn5 76.18(5) . 52_566
Sn4 Ba1 Sn5 44.02(3) 10_656 52_566
Sn4 Ba1 Sn5 74.76(4) 2_665 52_566
Sn4 Ba1 Sn5 119.24(8) 6_566 52_566
Sn5 Ba1 Sn5 42.60(4) 92_566 52_566
Sn2 Ba1 Sn5 76.18(5) . 72_665
Sn4 Ba1 Sn5 44.01(3) 10_656 72_665
Sn4 Ba1 Sn5 119.24(8) 2_665 72_665
Sn4 Ba1 Sn5 74.76(4) 6_566 72_665
Sn5 Ba1 Sn5 114.48(4) 92_566 72_665
Sn5 Ba1 Sn5 73.49(4) 52_566 72_665
Sn2 Ba1 Sn5 76.18(5) . 80_656
Sn4 Ba1 Sn5 119.24(8) 10_656 80_656
Sn4 Ba1 Sn5 44.02(3) 2_665 80_656
Sn4 Ba1 Sn5 74.76(4) 6_566 80_656
Sn5 Ba1 Sn5 73.49(4) 92_566 80_656
Sn5 Ba1 Sn5 114.48(3) 52_566 80_656
Sn5 Ba1 Sn5 148.10(8) 72_665 80_656
Sn2 Ba1 Sn5 76.18(5) . 40_656
Sn4 Ba1 Sn5 119.24(8) 10_656 40_656
Sn4 Ba1 Sn5 74.76(4) 2_665 40_656
Sn4 Ba1 Sn5 44.01(3) 6_566 40_656
Sn5 Ba1 Sn5 114.48(3) 92_566 40_656
Sn5 Ba1 Sn5 148.10(8) 52_566 40_656
Sn5 Ba1 Sn5 114.48(4) 72_665 40_656
Sn5 Ba1 Sn5 42.60(4) 80_656 40_656
Sn2 Ba1 Sn5 76.18(5) . 36_665
Sn4 Ba1 Sn5 74.76(4) 10_656 36_665
Sn4 Ba1 Sn5 119.24(8) 2_665 36_665
Sn4 Ba1 Sn5 44.01(3) 6_566 36_665
Sn5 Ba1 Sn5 148.10(8) 92_566 36_665
Sn5 Ba1 Sn5 114.48(4) 52_566 36_665
Sn5 Ba1 Sn5 42.60(4) 72_665 36_665
Sn5 Ba1 Sn5 114.48(4) 80_656 36_665
Sn5 Ba1 Sn5 73.49(4) 40_656 36_665
Sn2 Ba1 Sn1 149.92(5) . 4_666
Sn4 Ba1 Sn1 114.47(5) 10_656 4_666
Sn4 Ba1 Sn1 114.47(5) 2_665 4_666
Sn4 Ba1 Sn1 163.60(8) 6_566 4_666
Sn5 Ba1 Sn1 75.84(6) 92_566 4_666
Sn5 Ba1 Sn1 75.84(6) 52_566 4_666
Sn5 Ba1 Sn1 105.95(4) 72_665 4_666
Sn5 Ba1 Sn1 105.95(4) 80_656 4_666
Sn5 Ba1 Sn1 126.16(7) 40_656 4_666
Sn5 Ba1 Sn1 126.16(6) 36_665 4_666
Sn2 Ba1 Sn1 149.92(6) . 2_666
Sn4 Ba1 Sn1 114.47(5) 10_656 2_666
Sn4 Ba1 Sn1 163.60(8) 2_665 2_666
Sn4 Ba1 Sn1 114.47(5) 6_566 2_666
Sn5 Ba1 Sn1 126.16(7) 92_566 2_666
Sn5 Ba1 Sn1 105.95(4) 52_566 2_666
Sn5 Ba1 Sn1 75.84(6) 72_665 2_666
Sn5 Ba1 Sn1 126.16(7) 80_656 2_666
Sn5 Ba1 Sn1 105.95(4) 40_656 2_666
Sn5 Ba1 Sn1 75.84(6) 36_665 2_666
Sn1 Ba1 Sn1 51.45(9) 4_666 2_666
Sn7B Na1 Sn7B 58.6(11) 69 77
Sn7B Na1 Sn7B 64.1(13) 69 70_565
Sn7B Na1 Sn7B 23.7(14) 77 70_565
Sn7B Na1 Sn7B 23.7(14) 69 78_556
Sn7B Na1 Sn7B 64.1(13) 77 78_556
Sn7B Na1 Sn7B 58.6(11) 70_565 78_556
Sn7B Na1 Sn7B 81.5(9) 69 89
Sn7B Na1 Sn7B 29.2(14) 77 89
Sn7B Na1 Sn7B 46.8(9) 70_565 89
Sn7B Na1 Sn7B 92.3(2) 78_556 89
Sn7B Na1 Sn7B 29.2(14) 69 49
Sn7B Na1 Sn7B 81.5(9) 77 49
Sn7B Na1 Sn7B 92.3(2) 70_565 49
Sn7B Na1 Sn7B 46.8(9) 78_556 49
Sn7B Na1 Sn7B 95.7(14) 89 49
Sn7B Na1 Sn7B 46.8(9) 69 92_556
Sn7B Na1 Sn7B 92.3(2) 77 92_556
Sn7B Na1 Sn7B 81.5(9) 70_565 92_556
Sn7B Na1 Sn7B 29.2(14) 78_556 92_556
Sn7B Na1 Sn7B 121.2(15) 89 92_556
Sn7B Na1 Sn7B 54.5(10) 49 92_556
Sn7B Na1 Sn7B 92.3(2) 69 52_565
Sn7B Na1 Sn7B 46.8(9) 77 52_565
Sn7B Na1 Sn7B 29.2(14) 70_565 52_565
Sn7B Na1 Sn7B 81.5(9) 78_556 52_565
Sn7B Na1 Sn7B 54.5(10) 89 52_565
Sn7B Na1 Sn7B 121.2(15) 49 52_565
Sn7B Na1 Sn7B 95.7(14) 92_556 52_565
Sn7B Na1 Sn7B 46.8(9) 69 38_655
Sn7B Na1 Sn7B 104.0(6) 77 38_655
Sn7B Na1 Sn7B 110.2(7) 70_565 38_655
Sn7B Na1 Sn7B 54.5(10) 78_556 38_655
Sn7B Na1 Sn7B 119.20(18) 89 38_655
Sn7B Na1 Sn7B 23.7(14) 49 38_655
Sn7B Na1 Sn7B 46.8(9) 92_556 38_655
Sn7B Na1 Sn7B 135.9(8) 52_565 38_655
Sn7B Na1 Sn7B 104.0(7) 69 34_655
Sn7B Na1 Sn7B 46.8(9) 77 34_655
Sn7B Na1 Sn7B 54.5(10) 70_565 34_655
Sn7B Na1 Sn7B 110.2(7) 78_556 34_655
Sn7B Na1 Sn7B 23.7(14) 89 34_655
Sn7B Na1 Sn7B 119.20(18) 49 34_655
Sn7B Na1 Sn7B 135.9(8) 92_556 34_655
Sn7B Na1 Sn7B 46.8(9) 52_565 34_655
Sn7B Na1 Sn7B 142.4(15) 38_655 34_655
Sn7B Na1 Sn7B 110.2(7) 69 40_655
Sn7B Na1 Sn7B 54.5(10) 77 40_655
Sn7B Na1 Sn7B 46.8(9) 70_565 40_655
Sn7B Na1 Sn7B 104.0(6) 78_556 40_655
Sn7B Na1 Sn7B 46.8(9) 89 40_655
Sn7B Na1 Sn7B 135.9(8) 49 40_655
Sn7B Na1 Sn7B 119.20(18) 92_556 40_655
Sn7B Na1 Sn7B 23.7(14) 52_565 40_655
Sn7B Na1 Sn7B 156.9(11) 38_655 40_655
Sn7B Na1 Sn7B 29.2(14) 34_655 40_655
Sn7B Na1 Sn7B 54.5(10) 69 36_655
Sn7B Na1 Sn7B 110.2(7) 77 36_655
Sn7B Na1 Sn7B 104.0(6) 70_565 36_655
Sn7B Na1 Sn7B 46.8(9) 78_556 36_655
Sn7B Na1 Sn7B 135.9(8) 89 36_655
Sn7B Na1 Sn7B 46.8(9) 49 36_655
Sn7B Na1 Sn7B 23.7(14) 92_556 36_655
Sn7B Na1 Sn7B 119.20(18) 52_565 36_655
Sn7B Na1 Sn7B 29.2(14) 38_655 36_655
Sn7B Na1 Sn7B 156.9(11) 34_655 36_655
Sn7B Na1 Sn7B 142.4(15) 40_655 36_655
Sn4 Na2 Sn4 108.5(10) 29 57
Sn4 Na2 Sn4 108.5(10) 29 73
Sn4 Na2 Sn4 108.5(10) 57 73
Sn4 Na2 Sn2 52.05(17) 29 28_566
Sn4 Na2 Sn2 125.6(4) 57 28_566
Sn4 Na2 Sn2 125.6(4) 73 28_566
Sn4 Na2 Sn2 125.6(4) 29 51_656
Sn4 Na2 Sn2 52.08(17) 57 51_656
Sn4 Na2 Sn2 125.6(4) 73 51_656
Sn2 Na2 Sn2 95.0(11) 28_566 51_656
Sn4 Na2 Sn2 125.6(4) 29 74_665
Sn4 Na2 Sn2 125.6(4) 57 74_665
Sn4 Na2 Sn2 52.08(17) 73 74_665
Sn2 Na2 Sn2 95.0(11) 28_566 74_665
Sn2 Na2 Sn2 95.0(11) 51_656 74_665
Sn4 Na2 Na5 64.78(16) 29 53
Sn4 Na2 Na5 166(2) 57 53
Sn4 Na2 Na5 64.80(16) 73 53
Sn2 Na2 Na5 61.1(4) 28_566 53
Sn2 Na2 Na5 141.8(18) 51_656 53
Sn2 Na2 Na5 61.1(4) 74_665 53
Sn4 Na2 Na5 64.78(16) 29 81
Sn4 Na2 Na5 64.80(16) 57 81
Sn4 Na2 Na5 166(2) 73 81
Sn2 Na2 Na5 61.1(4) 28_566 81
Sn2 Na2 Na5 61.1(4) 51_656 81
Sn2 Na2 Na5 141.8(18) 74_665 81
Na5 Na2 Na5 118.7(4) 53 81
Sn4 Na2 Na5 166(2) 29 25
Sn4 Na2 Na5 64.83(16) 57 25
Sn4 Na2 Na5 64.83(16) 73 25
Sn2 Na2 Na5 141.8(18) 28_566 25
Sn2 Na2 Na5 61.2(4) 51_656 25
Sn2 Na2 Na5 61.2(4) 74_665 25
Na5 Na2 Na5 118.7(4) 53 25
Na5 Na2 Na5 118.7(4) 81 25
Sn4 Na2 Na8 55.5(7) 29 57
Sn4 Na2 Na8 108.4(16) 57 57
Sn4 Na2 Na8 55.5(7) 73 57
Sn2 Na2 Na8 98.1(4) 28_566 57
Sn2 Na2 Na8 160.5(14) 51_656 57
Sn2 Na2 Na8 98.2(4) 74_665 57
Na5 Na2 Na8 57.7(6) 53 57
Na5 Na2 Na8 113.6(10) 81 57
Na5 Na2 Na8 113.6(10) 25 57
Sn4 Na2 Na8 55.5(7) 29 73
Sn4 Na2 Na8 55.5(7) 57 73
Sn4 Na2 Na8 108.4(16) 73 73
Sn2 Na2 Na8 98.1(4) 28_566 73
Sn2 Na2 Na8 98.2(4) 51_656 73
Sn2 Na2 Na8 160.5(14) 74_665 73
Na5 Na2 Na8 113.6(10) 53 73
Na5 Na2 Na8 57.7(6) 81 73
Na5 Na2 Na8 113.6(10) 25 73
Na8 Na2 Na8 65.7(10) 57 73
Sn4 Na2 Na8 108.4(16) 29 29
Sn4 Na2 Na8 55.6(7) 57 29
Sn4 Na2 Na8 55.6(7) 73 29
Sn2 Na2 Na8 160.4(14) 28_566 29
Sn2 Na2 Na8 98.2(4) 51_656 29
Sn2 Na2 Na8 98.2(4) 74_665 29
Na5 Na2 Na8 113.6(10) 53 29
Na5 Na2 Na8 113.6(10) 81 29
Na5 Na2 Na8 57.7(6) 25 29
Na8 Na2 Na8 65.8(10) 57 29
Na8 Na2 Na8 65.8(10) 73 29
Sn8 Na3 Sn3 130.8(4) . 5
Sn8 Na3 Sn3 130.8(4) . 9
Sn3 Na3 Sn3 82.0(6) 5 9
Sn8 Na3 Sn3 130.8(4) . .
Sn3 Na3 Sn3 82.0(6) 5 .
Sn3 Na3 Sn3 82.0(6) 9 .
Sn8 Na3 Sn1 180.0(5) . .
Sn3 Na3 Sn1 49.2(4) 5 .
Sn3 Na3 Sn1 49.2(4) 9 .
Sn3 Na3 Sn1 49.2(4) . .
Sn8 Na3 Sn10 24.7(5) . 66
Sn3 Na3 Sn10 107.1(6) 5 66
Sn3 Na3 Sn10 146.3(5) 9 66
Sn3 Na3 Sn10 130.9(5) . 66
Sn1 Na3 Sn10 155.3(5) . 66
Sn8 Na3 Sn10 24.7(5) . 74
Sn3 Na3 Sn10 107.1(6) 5 74
Sn3 Na3 Sn10 130.9(5) 9 74
Sn3 Na3 Sn10 146.3(5) . 74
Sn1 Na3 Sn10 155.3(5) . 74
Sn10 Na3 Sn10 15.5(6) 66 74
Sn8 Na3 Sn10 24.7(5) . 58
Sn3 Na3 Sn10 130.9(5) 5 58
Sn3 Na3 Sn10 146.3(5) 9 58
Sn3 Na3 Sn10 107.1(6) . 58
Sn1 Na3 Sn10 155.3(5) . 58
Sn10 Na3 Sn10 31.8(12) 66 58
Sn10 Na3 Sn10 42.4(9) 74 58
Sn8 Na3 Sn10 24.7(5) . 86
Sn3 Na3 Sn10 130.9(5) 5 86
Sn3 Na3 Sn10 107.1(6) 9 86
Sn3 Na3 Sn10 146.3(5) . 86
Sn1 Na3 Sn10 155.3(5) . 86
Sn10 Na3 Sn10 42.4(9) 66 86
Sn10 Na3 Sn10 31.8(12) 74 86
Sn10 Na3 Sn10 48.4(9) 58 86
Sn8 Na3 Sn10 24.7(5) . 46
Sn3 Na3 Sn10 146.3(5) 5 46
Sn3 Na3 Sn10 130.9(5) 9 46
Sn3 Na3 Sn10 107.1(6) . 46
Sn1 Na3 Sn10 155.3(5) . 46
Sn10 Na3 Sn10 42.4(9) 66 46
Sn10 Na3 Sn10 48.4(9) 74 46
Sn10 Na3 Sn10 15.5(6) 58 46
Sn10 Na3 Sn10 42.4(9) 86 46
Sn8 Na3 Sn10 24.7(5) . 30
Sn3 Na3 Sn10 146.3(5) 5 30
Sn3 Na3 Sn10 107.1(6) 9 30
Sn3 Na3 Sn10 130.9(5) . 30
Sn1 Na3 Sn10 155.3(5) . 30
Sn10 Na3 Sn10 48.4(9) 66 30
Sn10 Na3 Sn10 42.4(9) 74 30
Sn10 Na3 Sn10 42.4(9) 58 30
Sn10 Na3 Sn10 15.5(6) 86 30
Sn10 Na3 Sn10 31.8(12) 46 30
Sn8 Na3 Na7 69.8(5) . 5
Sn3 Na3 Na7 60.9(2) 5 5
Sn3 Na3 Na7 125.5(3) 9 5
Sn3 Na3 Na7 125.5(3) . 5
Sn1 Na3 Na7 110.2(5) . 5
Sn10 Na3 Na7 46.9(7) 66 5
Sn10 Na3 Na7 46.9(7) 74 5
Sn10 Na3 Na7 76.2(7) 58 5
Sn10 Na3 Na7 76.3(7) 86 5
Sn10 Na3 Na7 89.0(7) 46 5
Sn10 Na3 Na7 89.0(7) 30 5
Sn7A Na4 Sn7A 57.4(5) 30 29_544
Sn7A Na4 Sn3 178.9(4) 30 6
Sn7A Na4 Sn3 123.77(8) 29_544 6
Sn7A Na4 Sn3 123.77(8) 30 5
Sn7A Na4 Sn3 178.9(4) 29_544 5
Sn3 Na4 Sn3 55.1(4) 6 5
Sn7A Na4 Sn7B 10.8(6) 30 96
Sn7A Na4 Sn7B 55.6(6) 29_544 96
Sn3 Na4 Sn7B 169.4(6) 6 96
Sn3 Na4 Sn7B 125.5(5) 5 96
Sn7A Na4 Sn7B 10.8(6) 30 56
Sn7A Na4 Sn7B 55.6(6) 29_544 56
Sn3 Na4 Sn7B 169.4(6) 6 56
Sn3 Na4 Sn7B 125.5(5) 5 56
Sn7B Na4 Sn7B 21.1(11) 96 56
Sn7A Na4 Sn7B 55.6(6) 30 95_545
Sn7A Na4 Sn7B 10.8(6) 29_544 95_545
Sn3 Na4 Sn7B 125.5(5) 6 95_545
Sn3 Na4 Sn7B 169.4(6) 5 95_545
Sn7B Na4 Sn7B 56.2(10) 96 95_545
Sn7B Na4 Sn7B 51.5(10) 56 95_545
Sn7A Na4 Sn7B 55.6(6) 30 55_554
Sn7A Na4 Sn7B 10.8(6) 29_544 55_554
Sn3 Na4 Sn7B 125.5(5) 6 55_554
Sn3 Na4 Sn7B 169.4(6) 5 55_554
Sn7B Na4 Sn7B 51.5(10) 96 55_554
Sn7B Na4 Sn7B 56.2(10) 56 55_554
Sn7B Na4 Sn7B 21.1(11) 95_545 55_554
Sn7A Na4 Na7 57.0(3) 30 5
Sn7A Na4 Na7 114.3(7) 29_544 5
Sn3 Na4 Na7 121.9(7) 6 5
Sn3 Na4 Na7 66.8(3) 5 5
Sn7B Na4 Na7 60.0(6) 96 5
Sn7B Na4 Na7 60.0(6) 56 5
Sn7B Na4 Na7 111.5(8) 95_545 5
Sn7B Na4 Na7 111.5(8) 55_554 5
Sn7A Na4 Na7 114.3(7) 30 6
Sn7A Na4 Na7 57.0(3) 29_544 6
Sn3 Na4 Na7 66.8(3) 6 6
Sn3 Na4 Na7 121.9(7) 5 6
Sn7B Na4 Na7 111.5(8) 96 6
Sn7B Na4 Na7 111.5(8) 56 6
Sn7B Na4 Na7 60.0(6) 95_545 6
Sn7B Na4 Na7 60.0(6) 55_554 6
Na7 Na4 Na7 171.3(10) 5 6
Sn7A Na4 Sn5 130.7(4) 30 39
Sn7A Na4 Sn5 91.99(18) 29_544 39
Sn3 Na4 Sn5 49.9(2) 6 39
Sn3 Na4 Sn5 87.2(5) 5 39
Sn7B Na4 Sn5 138.1(7) 96 39
Sn7B Na4 Sn5 120.3(7) 56 39
Sn7B Na4 Sn5 86.9(5) 95_545 39
Sn7B Na4 Sn5 100.7(6) 55_554 39
Na7 Na4 Sn5 132.1(3) 5 39
Na7 Na4 Sn5 52.29(15) 6 39
Sn7A Na4 Sn5 130.7(4) 30 35
Sn7A Na4 Sn5 91.99(18) 29_544 35
Sn3 Na4 Sn5 49.9(2) 6 35
Sn3 Na4 Sn5 87.2(5) 5 35
Sn7B Na4 Sn5 120.3(7) 96 35
Sn7B Na4 Sn5 138.1(7) 56 35
Sn7B Na4 Sn5 100.7(6) 95_545 35
Sn7B Na4 Sn5 86.9(5) 55_554 35
Na7 Na4 Sn5 132.1(3) 5 35
Na7 Na4 Sn5 52.30(15) 6 35
Sn5 Na4 Sn5 82.3(3) 39 35
Na2 Na5 Na2 84(2) 4_566 25_544
Na2 Na5 Sn2 58.9(6) 4_566 50_664
Na2 Na5 Sn2 58.9(6) 25_544 50_664
Na2 Na5 Sn2 58.9(6) 4_566 75_646
Na2 Na5 Sn2 58.9(6) 25_544 75_646
Sn2 Na5 Sn2 92.2(5) 50_664 75_646
Na2 Na5 Sn4 53.7(5) 4_566 76_556
Na2 Na5 Sn4 106.8(8) 25_544 76_556
Sn2 Na5 Sn4 112.3(5) 50_664 76_556
Sn2 Na5 Sn4 48.54(15) 75_646 76_556
Na2 Na5 Sn4 53.7(5) 4_566 59_565
Na2 Na5 Sn4 106.8(8) 25_544 59_565
Sn2 Na5 Sn4 48.54(15) 50_664 59_565
Sn2 Na5 Sn4 112.3(5) 75_646 59_565
Sn4 Na5 Sn4 92.57(17) 76_556 59_565
Na2 Na5 Sn4 106.8(8) 4_566 49_554
Na2 Na5 Sn4 53.7(5) 25_544 49_554
Sn2 Na5 Sn4 48.54(15) 50_664 49_554
Sn2 Na5 Sn4 112.3(5) 75_646 49_554
Sn4 Na5 Sn4 156.5(7) 76_556 49_554
Sn4 Na5 Sn4 82.65(14) 59_565 49_554
Na2 Na5 Sn4 106.8(8) 4_566 81_545
Na2 Na5 Sn4 53.7(5) 25_544 81_545
Sn2 Na5 Sn4 112.3(5) 50_664 81_545
Sn2 Na5 Sn4 48.54(15) 75_646 81_545
Sn4 Na5 Sn4 82.65(14) 76_556 81_545
Sn4 Na5 Sn4 156.5(7) 59_565 81_545
Sn4 Na5 Sn4 92.57(17) 49_554 81_545
Na2 Na5 Na6 138.2(10) 4_566 74
Na2 Na5 Na6 138.2(10) 25_544 74
Sn2 Na5 Na6 133.9(3) 50_664 74
Sn2 Na5 Na6 133.9(3) 75_646 74
Sn4 Na5 Na6 101.8(3) 76_556 74
Sn4 Na5 Na6 101.8(3) 59_565 74
Sn4 Na5 Na6 101.8(3) 49_554 74
Sn4 Na5 Na6 101.8(3) 81_545 74
Na2 Na5 Sn5 132.82(18) 4_566 26_654
Na2 Na5 Sn5 98.7(7) 25_544 26_654
Sn2 Na5 Sn5 155.8(2) 50_664 26_654
Sn2 Na5 Sn5 81.97(7) 75_646 26_654
Sn4 Na5 Sn5 81.26(12) 76_556 26_654
Sn4 Na5 Sn5 154.5(5) 59_565 26_654
Sn4 Na5 Sn5 112.26(19) 49_554 26_654
Sn4 Na5 Sn5 47.47(7) 81_545 26_654
Na6 Na5 Sn5 56.2(3) 74 26_654
Na2 Na5 Sn5 132.82(18) 4_566 42_645
Na2 Na5 Sn5 98.7(7) 25_544 42_645
Sn2 Na5 Sn5 81.97(7) 50_664 42_645
Sn2 Na5 Sn5 155.8(2) 75_646 42_645
Sn4 Na5 Sn5 154.5(5) 76_556 42_645
Sn4 Na5 Sn5 81.26(12) 59_565 42_645
Sn4 Na5 Sn5 47.47(7) 49_554 42_645
Sn4 Na5 Sn5 112.26(19) 81_545 42_645
Na6 Na5 Sn5 56.2(3) 74 42_645
Sn5 Na5 Sn5 93.7(4) 26_654 42_645
Na2 Na5 Sn5 98.7(7) 4_566 3_656
Na2 Na5 Sn5 132.82(18) 25_544 3_656
Sn2 Na5 Sn5 81.97(7) 50_664 3_656
Sn2 Na5 Sn5 155.8(2) 75_646 3_656
Sn4 Na5 Sn5 112.26(19) 76_556 3_656
Sn4 Na5 Sn5 47.47(7) 59_565 3_656
Sn4 Na5 Sn5 81.26(12) 49_554 3_656
Sn4 Na5 Sn5 154.5(5) 81_545 3_656
Na6 Na5 Sn5 56.2(3) 74 3_656
Sn5 Na5 Sn5 112.3(6) 26_654 3_656
Sn5 Na5 Sn5 46.75(17) 42_645 3_656
Sn10 Na6 Sn10 39(2) 21 5
Sn10 Na6 Sn10 50.6(9) 21 46
Sn10 Na6 Sn10 30(2) 5 46
Sn10 Na6 Sn10 30(2) 21 30
Sn10 Na6 Sn10 50.6(9) 5 30
Sn10 Na6 Sn10 39(2) 46 30
Sn10 Na6 Sn5 140.4(10) 21 89_445
Sn10 Na6 Sn5 119.1(14) 5 89_445
Sn10 Na6 Sn5 94.5(5) 46 89_445
Sn10 Na6 Sn5 111.3(12) 30 89_445
Sn10 Na6 Sn5 119.1(14) 21 49_454
Sn10 Na6 Sn5 140.4(10) 5 49_454
Sn10 Na6 Sn5 111.3(12) 46 49_454
Sn10 Na6 Sn5 94.5(5) 30 49_454
Sn5 Na6 Sn5 49.9(3) 89_445 49_454
Sn10 Na6 Sn5 111.3(12) 21 76_456
Sn10 Na6 Sn5 94.5(5) 5 76_456
Sn10 Na6 Sn5 119.1(14) 46 76_456
Sn10 Na6 Sn5 140.4(10) 30 76_456
Sn5 Na6 Sn5 101.7(7) 89_445 76_456
Sn5 Na6 Sn5 123.9(11) 49_454 76_456
Sn10 Na6 Sn5 94.5(5) 21 68_465
Sn10 Na6 Sn5 111.3(12) 5 68_465
Sn10 Na6 Sn5 140.4(10) 46 68_465
Sn10 Na6 Sn5 119.1(14) 30 68_465
Sn5 Na6 Sn5 123.9(11) 89_445 68_465
Sn5 Na6 Sn5 101.7(7) 49_454 68_465
Sn5 Na6 Sn5 49.9(3) 76_456 68_465
Sn10 Na6 Na5 154.7(4) 21 74
Sn10 Na6 Na5 154.7(4) 5 74
Sn10 Na6 Na5 154.7(4) 46 74
Sn10 Na6 Na5 154.7(4) 30 74
Sn5 Na6 Na5 62.0(6) 89_445 74
Sn5 Na6 Na5 62.0(6) 49_454 74
Sn5 Na6 Na5 62.0(6) 76_456 74
Sn5 Na6 Na5 62.0(6) 68_465 74
Sn10 Na6 Na7 85.0(14) 21 35
Sn10 Na6 Na7 50.2(5) 5 35
Sn10 Na6 Na7 68.2(14) 46 35
Sn10 Na6 Na7 100.5(9) 30 35
Sn5 Na6 Na7 99.8(2) 89_445 35
Sn5 Na6 Na7 149.5(5) 49_454 35
Sn5 Na6 Na7 51.44(19) 76_456 35
Sn5 Na6 Na7 94.0(2) 68_465 35
Na5 Na6 Na7 104.7(6) 74 35
Sn10 Na6 Na7 50.2(5) 21 28
Sn10 Na6 Na7 85.0(14) 5 28
Sn10 Na6 Na7 100.5(9) 46 28
Sn10 Na6 Na7 68.2(14) 30 28
Sn5 Na6 Na7 149.5(5) 89_445 28
Sn5 Na6 Na7 99.8(2) 49_454 28
Sn5 Na6 Na7 94.0(2) 76_456 28
Sn5 Na6 Na7 51.44(19) 68_465 28
Na5 Na6 Na7 104.7(6) 74 28
Na7 Na6 Na7 110.4(6) 35 28
Sn10 Na6 Na7 68.2(14) 21 9
Sn10 Na6 Na7 100.5(9) 5 9
Sn10 Na6 Na7 85.0(14) 46 9
Sn10 Na6 Na7 50.2(5) 30 9
Sn5 Na6 Na7 94.0(2) 89_445 9
Sn5 Na6 Na7 51.44(19) 49_454 9
Sn5 Na6 Na7 149.5(5) 76_456 9
Sn5 Na6 Na7 99.8(2) 68_465 9
Na5 Na6 Na7 104.7(6) 74 9
Na7 Na6 Na7 150.6(11) 35 9
Na7 Na6 Na7 61.5(4) 28 9
Sn10 Na7 Sn10 18.8(5) 58 46
Sn10 Na7 Sn7A 145.0(13) 58 74
Sn10 Na7 Sn7A 145.1(13) 46 74
Sn10 Na7 Sn5 97.4(9) 58 77_445
Sn10 Na7 Sn5 112.0(9) 46 77_445
Sn7A Na7 Sn5 97.3(4) 74 77_445
Sn10 Na7 Sn5 112.0(9) 58 89_445
Sn10 Na7 Sn5 97.4(9) 46 89_445
Sn7A Na7 Sn5 97.3(4) 74 89_445
Sn5 Na7 Sn5 97.5(4) 77_445 89_445
Sn10 Na7 Sn9 23.6(13) 58 74
Sn10 Na7 Sn9 23.6(13) 46 74
Sn7A Na7 Sn9 124.4(5) 74 74
Sn5 Na7 Sn9 117.5(4) 77_445 74
Sn5 Na7 Sn9 117.5(4) 89_445 74
Sn10 Na7 Sn7B 136.1(13) 58 28
Sn10 Na7 Sn7B 141.2(14) 46 28
Sn7A Na7 Sn7B 11.7(6) 74 28
Sn5 Na7 Sn7B 93.0(5) 77_445 28
Sn5 Na7 Sn7B 108.7(7) 89_445 28
Sn9 Na7 Sn7B 118.3(7) 74 28
Sn10 Na7 Sn7B 141.2(14) 58 64
Sn10 Na7 Sn7B 136.1(13) 46 64
Sn7A Na7 Sn7B 11.7(6) 74 64
Sn5 Na7 Sn7B 108.7(7) 77_445 64
Sn5 Na7 Sn7B 93.0(5) 89_445 64
Sn9 Na7 Sn7B 118.3(7) 74 64
Sn7B Na7 Sn7B 20.6(11) 28 64
Sn10 Na7 Na4 159.9(13) 58 9
Sn10 Na7 Na4 159.9(13) 46 9
Sn7A Na7 Na4 51.6(5) 74 9
Sn5 Na7 Na4 64.6(3) 77_445 9
Sn5 Na7 Na4 64.6(3) 89_445 9
Sn9 Na7 Na4 176.1(7) 74 9
Sn7B Na7 Na4 57.8(7) 28 9
Sn7B Na7 Na4 57.8(7) 64 9
Sn10 Na7 Sn3 111.9(13) 58 .
Sn10 Na7 Sn3 111.9(13) 46 .
Sn7A Na7 Sn3 101.7(4) 74 .
Sn5 Na7 Sn3 48.74(18) 77_445 .
Sn5 Na7 Sn3 48.74(18) 89_445 .
Sn9 Na7 Sn3 133.9(5) 74 .
Sn7B Na7 Sn3 107.0(6) 28 .
Sn7B Na7 Sn3 107.0(6) 64 .
Na4 Na7 Sn3 50.0(4) 9 .
Sn10 Na7 Na8 108.0(5) 58 35
Sn10 Na7 Na8 125.6(7) 46 35
Sn7A Na7 Na8 57.1(3) 74 35
Sn5 Na7 Na8 55.7(3) 77_445 35
Sn5 Na7 Na8 134.4(5) 89_445 35
Sn9 Na7 Na8 107.9(3) 74 35
Sn7B Na7 Na8 47.0(6) 28 35
Sn7B Na7 Na8 67.6(7) 64 35
Na4 Na7 Na8 70.3(4) 9 35
Sn3 Na7 Na8 96.2(3) . 35
Sn10 Na7 Na8 125.6(7) 58 56
Sn10 Na7 Na8 108.0(5) 46 56
Sn7A Na7 Na8 57.1(3) 74 56
Sn5 Na7 Na8 134.4(5) 77_445 56
Sn5 Na7 Na8 55.7(3) 89_445 56
Sn9 Na7 Na8 107.9(3) 74 56
Sn7B Na7 Na8 67.6(7) 28 56
Sn7B Na7 Na8 47.0(6) 64 56
Na4 Na7 Na8 70.3(4) 9 56
Sn3 Na7 Na8 96.2(3) . 56
Na8 Na7 Na8 114.2(7) 35 56
Sn6 Na8 Sn7B 52.8(7) 73_445 5
Sn6 Na8 Sn7B 52.8(7) 73_445 17
Sn7B Na8 Sn7B 30.2(14) 5 17
Sn6 Na8 Sn5 128.5(3) 73_445 82_546
Sn7B Na8 Sn5 101.1(8) 5 82_546
Sn7B Na8 Sn5 126.8(8) 17 82_546
Sn6 Na8 Sn5 128.5(3) 73_445 94_456
Sn7B Na8 Sn5 126.8(8) 5 94_456
Sn7B Na8 Sn5 101.1(8) 17 94_456
Sn5 Na8 Sn5 102.9(5) 82_546 94_456
Sn6 Na8 Sn4 93.4(4) 73_445 53_455
Sn7B Na8 Sn4 109.7(7) 5 53_455
Sn7B Na8 Sn4 136.7(9) 17 53_455
Sn5 Na8 Sn4 50.22(15) 82_546 53_455
Sn5 Na8 Sn4 122.2(5) 94_456 53_455
Sn6 Na8 Sn4 93.4(4) 73_445 33_545
Sn7B Na8 Sn4 136.7(9) 5 33_545
Sn7B Na8 Sn4 109.7(7) 17 33_545
Sn5 Na8 Sn4 122.2(5) 82_546 33_545
Sn5 Na8 Sn4 50.22(15) 94_456 33_545
Sn4 Na8 Sn4 97.1(5) 53_455 33_545
Sn6 Na8 Sn7A 60.5(4) 73_445 79
Sn7B Na8 Sn7A 11.0(7) 5 79
Sn7B Na8 Sn7A 40.1(8) 17 79
Sn5 Na8 Sn7A 90.1(2) 82_546 79
Sn5 Na8 Sn7A 130.6(5) 94_456 79
Sn4 Na8 Sn7A 102.9(2) 53_455 79
Sn4 Na8 Sn7A 147.7(5) 33_545 79
Sn6 Na8 Sn7A 60.5(4) 73_445 84
Sn7B Na8 Sn7A 40.1(8) 5 84
Sn7B Na8 Sn7A 11.0(7) 17 84
Sn5 Na8 Sn7A 130.6(5) 82_546 84
Sn5 Na8 Sn7A 90.1(2) 94_456 84
Sn4 Na8 Sn7A 147.7(5) 53_455 84
Sn4 Na8 Sn7A 102.9(2) 33_545 84
Sn7A Na8 Sn7A 49.1(3) 79 84
Sn6 Na8 Na5 136.8(7) 73_445 9
Sn7B Na8 Na5 163.0(8) 5 9
Sn7B Na8 Na5 163.0(8) 17 9
Sn5 Na8 Na5 61.9(3) 82_546 9
Sn5 Na8 Na5 61.9(3) 94_456 9
Sn4 Na8 Na5 60.3(3) 53_455 9
Sn4 Na8 Na5 60.3(3) 33_545 9
Sn7A Na8 Na5 152.0(4) 79 9
Sn7A Na8 Na5 152.0(4) 84 9
Sn6 Na8 Na7 111.7(5) 73_445 56
Sn7B Na8 Na7 60.6(7) 5 56
Sn7B Na8 Na7 77.1(7) 17 56
Sn5 Na8 Na7 52.0(3) 82_546 56
Sn5 Na8 Na7 101.2(5) 94_456 56
Sn4 Na8 Na7 95.7(3) 53_455 56
Sn4 Na8 Na7 151.0(6) 33_545 56
Sn7A Na8 Na7 51.5(3) 79 56
Sn7A Na8 Na7 78.9(4) 84 56
Na5 Na8 Na7 105.0(6) 9 56
Sn6 Na8 Na7 111.7(5) 73_445 35
Sn7B Na8 Na7 77.1(7) 5 35
Sn7B Na8 Na7 60.5(7) 17 35
Sn5 Na8 Na7 101.2(5) 82_546 35
Sn5 Na8 Na7 52.0(3) 94_456 35
Sn4 Na8 Na7 151.0(6) 53_455 35
Sn4 Na8 Na7 95.7(3) 33_545 35
Sn7A Na8 Na7 78.9(4) 79 35
Sn7A Na8 Na7 51.5(3) 84 35
Na5 Na8 Na7 105.0(6) 9 35
Na7 Na8 Na7 62.3(5) 56 35
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sn1 Sn3 2.897(3) 5
Sn1 Sn3 2.897(3) 9
Sn1 Sn3 2.897(3) .
Sn1 Na3 3.60(3) .
Sn1 Ba1 4.010(3) 3_646
Sn1 Ba1 4.010(3) 2_664
Sn1 Ba1 4.010(3) 4_466
Sn2 Sn4 2.920(3) 10_656
Sn2 Sn4 2.920(3) 2_665
Sn2 Sn4 2.920(3) 6_566
Sn2 Na2 3.44(3) 51_656
Sn2 Na2 3.44(3) 74_665
Sn2 Na2 3.44(3) 28_566
Sn2 Na5 3.520(15) 50_665
Sn2 Na5 3.520(15) 34_656
Sn2 Na5 3.520(15) 78_566
Sn2 Ba1 3.625(5) .
Sn3 Sn3 2.898(4) 2
Sn3 Sn5 2.9252(17) 77_445
Sn3 Sn5 2.9252(17) 89_445
Sn3 Na4 3.13(2) 9
Sn3 Na3 3.33(2) .
Sn3 Na7 3.758(14) .
Sn4 Sn5 2.907(2) 78_456
Sn4 Sn5 2.907(2) 90_546
Sn4 Sn2 2.920(3) 2_665
Sn4 Na2 3.19(2) 73_445
Sn4 Na8 3.455(12) 33_545
Sn4 Na8 3.455(12) 53_455
Sn4 Na5 3.582(5) 29_545
Sn4 Na5 3.582(5) 49_455
Sn4 Ba1 3.767(3) 2_665
Sn5 Sn5 2.887(3) 41_545
Sn5 Sn4 2.907(2) 60_565
Sn5 Sn3 2.9252(17) 57
Sn5 Na7 3.238(9) 57
Sn5 Na8 3.394(12) 31_655
Sn5 Na6 3.424(18) 49
Sn5 Na5 3.638(12) 26_655
Sn5 Na4 3.697(10) 53
Sn5 Ba1 3.9740(16) 52_466
Sn6 Sn7B 2.67(4) 69
Sn6 Sn7B 2.67(4) 77
Sn6 Sn7B 2.67(4) 89
Sn6 Sn7B 2.67(4) 49
Sn6 Sn7B 2.67(4) 37
Sn6 Sn7B 2.67(4) 33
Sn6 Na8 3.00(2) 57
Sn6 Na8 3.00(2) 73
Sn6 Na8 3.00(2) 29
Sn6 Sn7A 3.280(6) 7_665
Sn6 Sn7A 3.280(6) 8_656
Sn6 Sn7A 3.280(6) 12_665
Sn7A Sn7B 0.77(4) 39
Sn7A Sn7B 0.77(4) 51
Sn7A Sn7B 2.26(4) 35
Sn7A Sn7B 2.26(4) 71
Sn7A Sn7A 2.879(8) 9
Sn7A Sn7A 2.879(8) 5
Sn7A Sn7A 2.898(8) 2_665
Sn7A Sn7B 2.96(3) 91
Sn7A Sn7B 2.96(3) 79
Sn7A Na4 3.02(2) 81
Sn7A Sn7B 3.06(3) 52_565
Sn7A Sn7B 3.06(3) 40_655
Sn7B Sn7A 0.77(4) 51
Sn7B Sn7B 1.28(7) 86
Sn7B Sn7B 1.56(8) 21
Sn7B Sn7A 2.26(4) 56
Sn7B Sn7B 2.46(5) 84
Sn7B Sn7B 2.46(5) 30
Sn7B Sn6 2.67(4) 49_454
Sn7B Sn7B 2.84(5) 44
Sn7B Sn7A 2.96(3) 58
Sn7B Na8 3.00(3) 9
Sn7B Sn7B 3.03(6) 85_455
Sn7B Sn7A 3.06(3) 52_465
Sn8 Sn10 1.65(6) 66
Sn8 Sn10 1.65(6) 74
Sn8 Sn10 1.65(6) 86
Sn8 Sn10 1.65(6) 58
Sn8 Sn10 1.65(6) 30
Sn8 Sn10 1.65(6) 46
Sn8 Sn9 2.712(12) 28
Sn8 Sn9 2.712(12) 74
Sn8 Sn9 2.712(12) 51
Sn8 Na3 2.83(3) .
Sn8 Sn10 2.97(3) 9
Sn8 Sn10 2.97(3) 13
Sn9 Sn10 1.36(7) 79
Sn9 Sn10 1.36(7) 71
Sn9 Sn10 1.36(7) 35
Sn9 Sn10 1.36(7) 39
Sn9 Sn10 1.36(7) 91
Sn9 Sn10 1.36(7) 51
Sn9 Sn8 2.712(12) 51
Sn9 Sn8 2.712(12) 74
Sn9 Sn8 2.712(12) 28
Sn9 Sn10 3.11(3) 96
Sn9 Sn10 3.11(3) 56
Sn9 Sn10 3.11(3) 44
Sn10 Sn10 1.01(3) 44
Sn10 Sn9 1.36(7) 51
Sn10 Sn10 1.59(10) 86
Sn10 Sn8 1.65(6) 74
Sn10 Sn10 2.04(10) 13
Sn10 Sn10 2.27(10) 84
Sn10 Sn10 2.27(10) 30
Sn10 Sn10 2.59(4) 74
Sn10 Sn10 2.60(11) 21
Sn10 Sn10 2.69(9) 56
Sn10 Sn10 2.69(9) 35
Ba1 Sn4 3.767(3) 10_656
Ba1 Sn4 3.767(3) 2_665
Ba1 Sn4 3.767(3) 6_566
Ba1 Sn5 3.9739(17) 92_566
Ba1 Sn5 3.9739(17) 52_566
Ba1 Sn5 3.9739(17) 72_665
Ba1 Sn5 3.9740(16) 80_656
Ba1 Sn5 3.9740(17) 40_656
Ba1 Sn5 3.9740(17) 36_665
Ba1 Sn1 4.010(3) 4_666
Ba1 Sn1 4.010(3) 2_666
Na1 Sn7B 3.10(3) 69
Na1 Sn7B 3.10(3) 77
Na1 Sn7B 3.10(3) 70_565
Na1 Sn7B 3.10(3) 78_556
Na1 Sn7B 3.10(3) 89
Na1 Sn7B 3.10(3) 49
Na1 Sn7B 3.10(3) 92_556
Na1 Sn7B 3.10(3) 52_565
Na1 Sn7B 3.10(3) 38_655
Na1 Sn7B 3.10(3) 34_655
Na1 Sn7B 3.10(3) 40_655
Na1 Sn7B 3.10(3) 36_655
Na2 Sn4 3.19(2) 29
Na2 Sn4 3.19(2) 57
Na2 Sn4 3.19(2) 73
Na2 Sn2 3.44(3) 28_566
Na2 Sn2 3.44(3) 51_656
Na2 Sn2 3.44(3) 74_665
Na2 Na5 3.480(18) 53
Na2 Na5 3.480(18) 81
Na2 Na5 3.478(18) 25
Na2 Na8 4.05(5) 57
Na2 Na8 4.05(5) 73
Na2 Na8 4.04(5) 29
Na3 Sn3 3.33(2) 5
Na3 Sn3 3.33(2) 9
Na3 Sn10 3.72(7) 66
Na3 Sn10 3.72(7) 74
Na3 Sn10 3.72(7) 58
Na3 Sn10 3.72(7) 86
Na3 Sn10 3.72(7) 46
Na3 Sn10 3.72(7) 30
Na3 Na7 3.995(19) 5
Na4 Sn7A 3.02(2) 30
Na4 Sn7A 3.02(2) 29_544
Na4 Sn3 3.13(2) 6
Na4 Sn3 3.13(2) 5
Na4 Sn7B 3.49(4) 96
Na4 Sn7B 3.49(4) 56
Na4 Sn7B 3.49(4) 95_545
Na4 Sn7B 3.49(4) 55_554
Na4 Na7 3.649(15) 5
Na4 Na7 3.649(15) 6
Na4 Sn5 3.697(10) 39
Na4 Sn5 3.697(10) 35
Na5 Na2 3.478(18) 4_566
Na5 Na2 3.478(18) 25_544
Na5 Sn2 3.520(15) 50_664
Na5 Sn2 3.520(15) 75_646
Na5 Sn4 3.582(5) 76_556
Na5 Sn4 3.582(5) 59_565
Na5 Sn4 3.582(5) 49_554
Na5 Sn4 3.582(5) 81_545
Na5 Na6 3.64(4) 74
Na5 Sn5 3.638(12) 26_654
Na5 Sn5 3.638(12) 42_645
Na5 Sn5 3.638(12) 3_656
Na6 Sn10 3.03(4) 21
Na6 Sn10 3.03(4) 5
Na6 Sn10 3.03(4) 46
Na6 Sn10 3.03(4) 30
Na6 Sn5 3.424(18) 89_445
Na6 Sn5 3.424(18) 49_454
Na6 Sn5 3.424(18) 76_456
Na6 Sn5 3.424(18) 68_465
Na6 Na5 3.64(4) 74
Na6 Na7 3.956(13) 35
Na6 Na7 3.955(13) 28
Na6 Na7 3.956(13) 9
Na7 Sn10 3.08(3) 58
Na7 Sn10 3.08(3) 46
Na7 Sn7A 3.229(17) 74
Na7 Sn5 3.238(9) 77_445
Na7 Sn5 3.238(9) 89_445
Na7 Sn9 3.390(19) 74
Na7 Sn7B 3.57(4) 28
Na7 Sn7B 3.57(4) 64
Na7 Na4 3.649(15) 9
Na7 Na8 3.912(19) 35
Na7 Na8 3.912(19) 56
Na8 Sn6 3.00(2) 73_445
Na8 Sn7B 3.00(3) 5
Na8 Sn7B 3.00(3) 17
Na8 Sn5 3.394(12) 82_546
Na8 Sn5 3.394(12) 94_456
Na8 Sn4 3.455(12) 53_455
Na8 Sn4 3.456(12) 33_545
Na8 Sn7A 3.466(17) 79
Na8 Sn7A 3.466(17) 84
Na8 Na5 3.67(2) 9
Na8 Na7 3.912(19) 56
Na8 Na7 3.912(19) 35
